# LS-DYNA Matematics Model

date post

18-Nov-2014Category

## Documents

view

800download

15

Embed Size (px)

### Transcript of LS-DYNA Matematics Model

Section 1. Theoretical Manual - Manual for LS-DYNA Wood Material...

file:///D:/Dragan/D%20I%20P%20L%20O%20M%20S%20K%20I/...

TFHRC Home > Safety > FHWA-HRT-04-097 > Theoretical Manual

>

Manual for LS-DYNA Wood Material Model 143Section 1. THEORETICAL MANUALThis section documents the theory of the wood material model in detail. It begins with an overview of wood behavior, followed by an overview of the formulation. Then detailed equations are provided for each feature of the model (elasticity, plasticity, hardening, damage, and rate effects). Data are also tabulated for southern yellow pine and Douglas fir that are needed to fit the model parameters. Throughout this report, numerous figures, particularly those of test data, are reproduced from the various references cited at the end of each caption. 1.1 BEHAVIOR OF WOOD Wood is a variable material; however, certain trends are evident. Stiffness and strength properties vary as a function of orientation between the longitudinal, tangential, and radial directions. Figure 1 helps to illustrate this point. The longitudinal direction is the fiber or grain direction. Stiffness and strength are greatest in the fiber direction. The tangential and radial directions are transverse to the fiber direction, and tangential and perpendicular to the growth rings. For modeling purposes, the distinction between the tangential and radial directions is not always significant. Therefore, this manual uses the term perpendicular to the grain when no distinction is made between the radial and tangential directions, and parallel to the grain to describe the longitudinal direction.

Figure 1. Wood material properties vary with orientation. The wood material coordinate system does not necessarily coincide with the board coordinate system. (6) Source: American Society of Civil Engineers. Loading wood at angles to the grain has a significant effect on strength, as demonstrated in figure 2 for Douglas fir. The data are indicated by the dots. Hankinsons formula is indicated by the surface. This formula is discussed in section 1.4.

1 of 9

16.12.2009 14:56

Section 1. Theoretical Manual - Manual for LS-DYNA Wood Material...

file:///D:/Dragan/D%20I%20P%20L%20O%20M%20S%20K%20I/...

Figure 2. Ultimate tensile strength of Douglas fir measured in off-axis tests drops rapidly as the load is oriented at increasing angles to the grain. Source: Society of Wood Science and Technology.(7) The failure modes and measured stress-strain relationships of wood depend on the direction of the load relative to the grain and the type of load (tension, compression, or shear). The stress-strain relationships of wood in parallel tension, perpendicular tension, and shear are typically linear to brittle failure, while the stress-strain relationships of wood in parallel compression and perpendicular compression are typically nonlinear and ductile. Another factor that affects the measured stress-strain relationships is moisture content. The stress-strain behavior of southern yellow pine in tension and compression is plotted in figure 3 as a function of moisture content. The data indicate a factor of up to three variations in strength with moisture content. The data also demonstrate brittle behavior in tension versus ductile behavior in compression. Saturation refers to the fiber saturation point, which is approximately 23 percent. The behavior in shear was not measured. It is important to distinguish between the modes of failure because the effect of each mode on the ultimate strength of the wood posts may be quite different. For example, impacted wood posts have been observed to fail by parallel tensile and shear mechanisms. Thus, ultimate wood post failure occurs in the brittle modes (parallel to the grain), not the ductile modes. It is possible for perpendicular yielding to precede parallel failure, but not be catastrophic.

Figure 3. Measured stress-strain relationships of southern yellow pine depend on load direction (parallel or perpendicular), load type (tensile or compressive), and moisture content.

2 of 9

16.12.2009 14:56

Section 1. Theoretical Manual - Manual for LS-DYNA Wood Material...

file:///D:/Dragan/D%20I%20P%20L%20O%20M%20S%20K%20I/...

Temperature also affects the behavior of wood. This is demonstrated in figure 4 for wood posts impacted by bogie vehicles at 9.4 meters per second (m/s). There is a difference of a factor of 3 in measured response (force and velocity) between the frozen and unfrozen posts, which are made of southern yellow pine. The measured response of the Douglas fir post lies between that of the frozen and unfrozen southern yellow pine posts. Wood exhibits progressive softening, as demonstrated by the splitting test data shown in figure 5 for southern yellow pine. In addition, wood exhibits modulus reduction and permanent plastic deformation, as demonstrated by the cyclic load curve shown in figure 6. Modulus reduction is indicated by the decrease in the elastic loading/unloading slopes as strain softening progresses. Permanent deformation is evident because the data unloads to zero stress at nonzero values of strain. The fracture area is the area under the load-displacement curve following peak stress. The data (8) were obtained from splitting tests conducted by Stanzl-Tschegg, et al. Although the data are for spruce wood, similar behavior is expected for pine and fir.

Figure 4. Temperature affects the dynamic behavior of wood posts impacted by bogies at 9.4 m/s.

3 of 9

16.12.2009 14:56

Section 1. Theoretical Manual - Manual for LS-DYNA Wood Material...

file:///D:/Dragan/D%20I%20P%20L%20O%20M%20S%20K%20I/...

Figure 5. (9) Wood exhibits progressive softening. Source: Forest Products Laboratory.

Figure 6. Wood exhibits modulus reduction and permanent deformation (splitting test data for spruce wood from Stanzi-Tschegg, et al.). (8) Source: Kluwer Academic Publishers, with the permission of Springer Science and Business Media. Wood is a variable material. The variability of the clear wood properties of southern yellow pine is given in figure 7 for tension parallel and compression perpendicular at 12 percent moisture content. The variability at other moisture contents is given in appendix A. Note that strength measurements vary by about a factor of 2 at each moisture content. In general, material properties vary as a function of position in a post, board, or test specimen. This is usually caused by natural variations in density; the presence of latewood and earlywood growth rings; and defects and growth characteristics, such as knots, checks, and shakes. Latewood is typically denser and stronger than earlywood. Knots, in particular, reduce the strength of wood. The reduction in strength depends on the knot size relative to the board size; the knot position (edge, center); and the wood parallel tensile strength, as shown in figure 8. Bogie impact tests indicate that the peak force in DS-65 posts is about 40 percent greater than that in grade 1 (10) posts. Finally, wood exhibits an increase in strength with strain rate. This is demonstrated in figure 9 for various wood (11) The stress ratio increases with impact velocity and is most pronounced in the perpendicular direction. The species. stress ratio is the dynamic-to-static ratio measured in the Hopkinson bar tests. Rate effects are important when modeling vehicle collisions into wooden roadside structures.

4 of 9

16.12.2009 14:56

Section 1. Theoretical Manual - Manual for LS-DYNA Wood Material...

file:///D:/Dragan/D%20I%20P%20L%20O%20M%20S%20K%20I/...

Figure 7. Variability of southern yellow pine clear wood data at 12-percent moisture content depends on load direction and type.

Figure 8. Wood material properties vary with position. Board strength depends on position and size of knot. Source: Society of Wood Science and Technology.(12)

5 of 9

16.12.2009 14:56

Section 1. Theoretical Manual - Manual for LS-DYNA Wood Material...

file:///D:/Dragan/D%20I%20P%20L%20O%20M%20S%20K%20I/...

Figure 9. Dynamic strength of wood increases with impact velocity in Hopkinson bar tests and is most pronounced in the perpendicular direction. (11) Source: Pergamon, Elsevier Science Ltd. 1.2 OVERVIEW OF FORMULATION The wood model consists of a number of formulations that are merged together to form a comprehensive model: Elastic constitutive equations. Failure criteria. Plastic flow. Hardening Postpeak softening. Strain-rate enhancement. Each of these formulations is discussed separately. The flowchart in figure 10 shows how each formulation interacts

6 of 9

16.12.2009 14:56

Section 1. Theoretical Manual - Manual for LS-DYNA Wood Material...

file:///D:/Dragan/D%20I%20P%20L%20O%20M%20S%20K%20I/...

with the others. Each formulation requires specific input parameters, such as stiffness, strength, and fracture energy. The main source of the material properties listed in this section and used as default input parameters is the data measured by Forests (13,14) FPL data are plotted in Products Laboratory (FPL) for southern yellow pine as a function of moisture content. appendix A. It is important to note that the FPL data are for clear wood (small specimens without defects such as knots), whereas real-world posts are graded wood (grades 3, 2, 1, or DS-65). Clear wood is stronger than graded wood. Nevertheless, the clear wood data are used as the basis for the default material properties. To account for strength reductions as a function of grade, reduction factors are applied to the clear wood strengths. Our reduction factor methodology is thoroughly discussed in section 1.12.

7 of 9

16.12.2009 14:56

Section 1. Theoretical Manual - Manual for LS-DYNA Wood Material...

file:///D:/Dragan/D%20I%20P%20L%20O%20M%20S%20K%20I/...

Figure 10. Organization of wood material model. > FHWA-HRT-04-097 TFHRC Home | FHWA Home | Feedback

8 of 9

16.12.2009 14:56

Section 1.11. Temperature Effects - Manual for LS-DYNA Wood Materi...

http://www.tfhrc.gov/safety/pubs/04097/sec1x1.htm

TFHRC Home > Safety > FHWA-HRT-04-097 > Temperature Effects

>

Manual for LS-DYNA Wood Material Model 1431.11 TEMPERATURE EFFECTSTypically, the moduli and strength of wood decrease as temperature increases. In addition, temperature interacts with (16) This figure indicates that the temperature moisture to influence the mechanical properties, as shown in figure 24. effects are more pronounced at high moisture content than at low moisture content. If the temperature change is not sustained, then the effect is reversiblethe moduli and strengths will return to their original value at their original temperature. If the temperature change is sustained, then the effect is permanent, at least at elevated temperatures. This is because chemical changes occur in wood with prolonged exposure to elevated temperatures that degrade the wood properties and produce large reductions in strength. Repeated exposure to elevated temperatures also has a cumulative effect. Guardrail posts may be exposed to extreme temperatures for prolonged periods of time. Guardrail posts in warm regions that are exposed to high temperatures for long periods of time will have different properties than those in cold regions of the country. In addition, bogie tests on guardrail posts indicate that energy absorption goes down when posts freeze. This was previously demonstrated in figure 4. Although these observations on guardrail posts suggest that mechanical properties are affected by temperature, no clear wood data are available for southern yellow pine or Douglas fir that document the effect. Thus, the data from Bodig and Jayne and the USDA Wood Handbook are used.(16,18)

Figure 24. Effect of temperature and moisture interaction on longitudinal modulus. Here, three methods are suggested for modeling temperature effects. One method takes regional variations into account through the selection of a predefined temperature exposure parameter tabulated by region. This method would vary the moduli, strengths, and fracture energies as a function of the temperature exposure parameter. However, this approach is not practical at this time because neither the regional data nor the clear wood data are available to develop such a detailed model. A second method specifies temperature effects by range. For example, three broad ranges could be modeled: Low temperatures (below freezing). Intermediate temperatures. High temperatures. The user would specify a flag that indicates one of the three ranges. This method is simple to implement and easy to use, but does not give the user many choices.

1 of 3

16.12.2009 15:05

Section 1.11. Temperature Effects - Manual for LS-DYNA Wood Materi...

http://www.tfhrc.gov/safety/pubs/04097/sec1x1.htm

A third method specifies the temperature directly. With this method, the room-temperature (20 C) properties are scaled up or down according to the temperature specified. If no temperature is specified, the temperature defaults to room temperature (20 C) and no scale factor is applied. This method is currently used for the default material properties. The following factor (FM) is implemented to scale the clear wood moduli as a function of input temperature (T):

where: Coefficient a1 (C-2) Coefficient a2 (C-2) Coefficient a3 (C ) Coefficient b1 (C-1) Coefficient b2 (C-1) Coefficient b3 (C-1)-2

= 0.0000000377625 = 0.000001416 = 0.0000003125 = 0.000004817 = 0.000109895 = 0.000875

All six coefficients (a1, a2, a3, b1, b2, and b3) are obtained from fits to the data previously shown in figure 24(a) for six wood species. Equations 95 through 97 are plotted in figure 24(b). The data indicate that the stiffness of the wood increases when frozen and decreases when heated.

Equation 98 is based on the data shown in figure 25. Figure 25 indicates that temperature has a stronger effect on strength than it has on stiffness. For temperatures below 20 C, the increase in strength is twice that modeled for the increase in moduli. For temperatures above 20 C, the decrease in strength is twice that modeled for the decrease in moduli. These plots are reproduced from the USDA Wood Handbook and are a composite of the results obtained from several studies.(18)

Figure 25. Temperature effects are more pronounced for the strength parallel to the grain than for the modulus parallel to the grain. Source: Forest Products Laboratory.(18) The wood data shown in figure 25 may seem inconsistent with the bogie test data previously shown in figure 4. The bogie data indicate that it takes less impact force to break a frozen wood post than a room-temperature post. This may be because frozen posts are more brittle than room-temperature posts, so temperature may affect fracture energy. The author is not aware of any fracture intensity or energy data for frozen pine or fir that demonstrate the effect of temperature, either parallel or perpendicular to the grain. Therefore, the perpendicular-to-the-grain energy is modeled independent of temperature (using the FPL quadratic equations). However, wood is expected to become more brittle as temperature decreases. Therefore, parallel to the grain, a reduction in fracture energy is modeled upon freezing and an increase in fracture energy is modeled upon heating.

2 of 3

16.12.2009 15:05

Section 1.11. Temperature Effects - Manual for LS-DYNA Wood Materi...

http://www.tfhrc.gov/safety/pubs/04097/sec1x1.htm

The variation in fracture energy with temperature is based on correlations of dynamic bogie impact with frozen and room-temperature grade 1 posts. Good frozen grade 1 correlations are obtained with a parallel-to-perpendicular energy ratio of 5, which is very brittle behavior. To accommodate variation with temperature, the default parallel-to-the-grain energies are modeled with a linear variation with temperature (T) between frozen and room-temperature values:

Here, T is the temperature in degrees Celsius (C) between 0 and 20 C, and room temperature is 20 C. For temperatures lower than 0 C, the frozen fracture energies are the default values. For temperatures higher than 20 C, the room-temperature fracture energies are the default values. > FHWA-HRT-04-097 TFHRC Home | FHWA Home | FeedbackUnited States Department of Transportation - Federal Highway Administration

3 of 3

16.12.2009 15:05

Section 1.12. Variability by Grade - Manual for LS-DYNA Wood Mater...

http://www.tfhrc.gov/safety/pubs/04097/sec1x2.htm

TFHRC Home > Safety > FHWA-HRT-04-097 > Variability by Grade

>

Manual for LS-DYNA Wood Material Model 1431.12 VARIABILITY BY GRADEVisual grading includes an assessment of wood defects. When analyzing structures such as guardrail posts, the exact position of the defects will not be known, except in highly controlled laboratory tests. Therefore, a practical approach for addressing defects is to modify the material properties globally as a function of visual grade. This approach requires the implementation of the grade as an input parameter. Four input options are available for modeling strength and stiffness reductions by grade. The four options are listed in table 17: Table 17. Input options for modeling strength reductions by grade. Reduction Factors User Input Grade QT 0.47 QT = 0 QC Ignored 1, 1D, 2, or 2D 0.40 QT = -1 QC Ignored QT = -2 QC Ignored 0.0 < QT 1.0 0.0 < QC 1.0 DS-65 or SEL STR Clear Wood 0.80 1.00 0.70 0.93 1.00 Fir Pine & Fir Pine & Fir QC 0.63 Wood Pine

User-Specified

QT

QC

Pine & Fir

The user may request clear, high-grade (DS-65 or Select Structural), or low-grade (grades 1, 1D, 2, or 2D) wood. This is because significant differences were noted between DS-65 posts and posts of all other grades (1, 1D, 2, and 2D) tested. The DS65 posts are significantly stronger than all other posts. In addition, there is no statistically significant difference in response among the other posts, although the dense posts (grades 1D and 2D) tend to absorb more energy than the low-density (grades 1 and 2) posts. Therefore, the posts can effectively be divided into two grades. Our approach is to implement global strength-reduction factors as a function of grade. Two factors must be applied. One factor, QT, reduces the tensile and shear strengths of clear wood; the other factor, QC, reduces the compressive strengths. The factors are simultaneously applied to the parallel and perpendicular strengths. In addition to applying the predefined quality factors by grade, the user may directly specify the tensile and compressive reduction factors between 0 and 1. The Standard Grading Rules Handbook for southern pine lumber indicates that the perpendicular-to-the-grain compressive strength of lumber does not always vary with grade (perpendicular tensile strengths are not reported).(26) Therefore, an input flag (IFAIL) is available to allow the user to apply the strength-reduction factors parallel to the grain, but not perpendicular to the grain. Although strength-reduction factors are a global approach for modeling strength and stiffness reductions caused by defects, the user may want to model local defects in detail. This can be done by the appropriate selection of mesh, local wood properties, and local grain orientation. The modeling of defects in an explicit manner is expected to be time-consuming to set up and may be computationally intensive to run.

>

1 of 2

16.12.2009 15:05

Section 2. User's Manual - Manual for LS-DYNA Wood Material Mode...

http://www.tfhrc.gov/safety/pubs/04097/sec20.htm

TFHRC Home > Safety > FHWA-HRT-04-097 > Users Manual

>

Manual for LS-DYNA Wood Material Model 1432. USERS MANUALThis section is intended to be a brief users manual for those users who want to run the model with a cursory, rather than indepth, understanding of the underlying theory and equations. This section includes a description of the LS-DYNA wood model input, a brief parameter description, and methods of fitting the parameters to data. This section concludes with a brief description of the wood model theory and an example output file.

2.1 LS-DYNA INPUT*MAT_WOOD_{OPTION} This is material type 143. This is a transversely isotropic material and is available for solid elements in LS-DYNA. The user has the option of inputting his or her own material properties ( option) or requesting default material properties for southern yellow pine (PINE) or Douglas fir (FIR). Options include: PINE FIR such that the keyword cards appear: *MAT_WOOD_PINE *MAT_WOOD_FIR *MAT_WOOD Define the following card for all options: Card Format Card 1 Variable Type 1 MID I 2 RO F 3 NPLOT I 4 ITERS I 5 IRATE I 6 GHARD F 7 IFAIL I 8

Define the following cards for the PINE and FIR options: Card 2 Variable Type 1 MC F 2 TEMP F 3 QT F 4 QC F 5 UNITS I 6 IQUAL I 7 8

Define the following cards for the option (do not define for PINE or FIR): Card 3 Variable Type Card 4 Variable Type Card 5 Variable Type Card 6 1 EL F 1 XT F 1 Gf I^ F 1 2 ET F 2 XC F 2 Gf II || F 2 3 GLT F 3 YT F 3 B F 3 4 GTR F 4 YC F 4 dmax|| F 4 5 nLT F 5 S|| F 5 Gf I^ F 5 6 7 8

6 S^ F 6 Gf II^ F 6

7

8

7 D F 7

8 dmax^ F 8

1 of 5

16.12.2009 15:06

Section 2. User's Manual - Manual for LS-DYNA Wood Material Mode...

http://www.tfhrc.gov/safety/pubs/04097/sec20.htm

Variable Type Card 7 Variable Type

h|| F 1 N|| F

hC|| F 2 c|| F

n|| F 3 N^ F

h^ F 4 c^ F

hC^ F 5

n^ F 6 7 8

Define for all options: Card 8 Variable Type Card 9 Variable Type Card 10 Variable Type Variable MID RO Mass density NPLOT Plotting options: EQ. 1: Maximum of parallel and perpendicular damage (default) EQ. 2: Perpendicular damage ITERS Number of plasticity algorithm iterations (default is one iteration; values greater than 1 are not recommended) IRATE Rate-effect options: EQ. 0: Rate-effect model turned off (default) EQ. 1: Rate-effect model turned on GHARD Perfect plasticity override (values greater than or equal to zero are allowed). Positive values model late-time hardening in compression (an increase in strength with increasing strain). A zero value models perfect plasticity (no increase in strength with increasing strain). The default is zero. IFAIL Erosion perpendicular to the grain: EQ. 0: No (default) EQ. 1: Yes (not recommended except for debugging) Define for PINE and FIR options: VariableDescription MC Percent moisture content (if left blank, moisture content defaults to saturated at 30 percent) TEMP Temperature in C (if left blank, temperature defaults to room temperature at 20 C) 1 AOPT I 1 XP F 1 D1 F Description Material identification (a unique number has to be chosen) 2 3 4 5 6 7 8

2 YP F 2 D2 F

3 ZP F 3 D3 F

4 A1 F 4

5 A2 F 5

6 A3 F 6

7

8

7

8

2 of 5

16.12.2009 15:06

Section 2. User's Manual - Manual for LS-DYNA Wood Material Mode...

http://www.tfhrc.gov/safety/pubs/04097/sec20.htm

VariableDescription QT Quality factor options (these quality factors reduce the clear wood tension/shear and compression strengths as a function of grade): EQ. 0: Grades 1, 1D, 2, 2D Predefined strength-reduction factors are: Pine: Fir: QT = 0.47 in tension/shear QC = 0.63 in compression QT = 0.40 in tension/shear QC = 0.70 in compression

EQ. -1:DS-65 or SEL STR Predefined strength-reduction factors are: QT = 0.80 in tension/shear QC = 0.93 in compression EQ. -2:Clear wood QT = 1.0 in tension/shear QC = 1.0 in compression GT. User-defined quality factor in tension (values greater than 0 and less than or equal to 1 are 0: expected; values greater than 1 are allowed, but may not be realistic. QC User-defined quality factor in compression (This input value is used if QT > 0. Values greater than 0 and less than or equal to 1 are expected. Values greater than 1 are allowed, but may not be realistic. If left blank when QT > 0, a default value of QC = QT is used.) Unit options: EQ. 0: gigapascals (GPa), mm, milliseconds (ms), kilograms per cubic millimeter (kg/mm3), kilonewtons (kN) 3 EQ. 1: MPa, ms, grams per cubic millimeter (g/mm ), newtons (N) EQ. 2: MPa, mm, s, megagrams per cubic millimeter (Mg/mm3), N 2 2 4 EQ. 3: lbf/inch , inch, s, pound second squared per inch to the fourth power (lb-s /inch ), pounds force (lbf) IQUAL Apply quality factors perpendicular to the grain: EQ. 0: Yes (default) EQ. 1: No Remarks: Material property data are for clear wood (small samples without defects such as knots), whereas real structures are composed of graded wood. Clear wood is stronger than graded wood. Quality factors (strength-reduction factors) are applied to the clear wood strengths to account for reductions in strength as a function of grade. One quality factor (QT) is applied to the tensile and shear strengths. A second quality factor (QC) is applied to the compressive strengths. As an option, predefined quality factors are provided based on correlations between LS-DYNA calculations and test data for pine and fir posts impacted by bogie vehicles. By default, quality factors are applied to the parallel strengths and to the perpendicular strengths. An option is available (IQUAL) to eliminate application perpendicular to the grain. Define for option only: Variable EL Description Parallel normal modulus

UNITS

3 of 5

16.12.2009 15:06

Section 2. User's Manual - Manual for LS-DYNA Wood Material Mode...

http://www.tfhrc.gov/safety/pubs/04097/sec20.htm

Variable ET GLT GTR nLT XT XC YT YC S|| S^ Gf I || Gf II || B

Description Perpendicular normal modulus Parallel shear modulus (GLR = GLT) Perpendicular shear modulus Parallel major Poissons ratio Parallel tensile strength Parallel compressive strength Perpendicular tensile strength Perpendicular compressive strength Parallel shear strength Perpendicular shear strength Parallel fracture energy in tension Parallel fracture energy in shear Parallel softening parameter

dmax|| Gf I ^ Gf II ^ D

Parallel maximum damage Perpendicular fracture energy in tension Perpendicular fracture energy in shear Perpendicular softening parameter

dmax^ h|| hc|| n|| h^ hc^

Perpendicular maximum damage Parallel fluidity parameter in tension/shear Parallel fluidity parameter in compression Parallel power Perpendicular fluidity parameter in tension/shear Perpendicular fluidity parameter in compression

4 of 5

16.12.2009 15:06

Section 2. User's Manual - Manual for LS-DYNA Wood Material Mode...

http://www.tfhrc.gov/safety/pubs/04097/sec20.htm

Variable n^ N|| c|| N^ c^

Description Perpendicular power Parallel hardening initiation Parallel hardening rate Perpendicular hardening initiation Perpendicular hardening rate

Define for all options: AOPT material axes option (see MAT_OPTIONTROPIC_ELASTIC for a more complete description): EQ. 0: Locally orthotropic with material axes determined by element EQ. 1: Locally orthotropic with material axes determined by a point in space and the global location of the element center; this is the a-direction EQ. 2: Globally orthotropic with material axes determined by vectors defined below, as with *DEFINE_COORDINATE_VECTOR XP, YP, ZP A1, A2, A3 D1, D2, D3 Coordinates of point p for AOPT = 1 Coordinates of vector a for AOPT = 2 Components of vector d for AOPT = 2

Remarks: One common option is AOPT = 2. The user defines vectors a and d. Typically, a is the parallelto-the-grain direction and d is one of the perpendicular-to-the-grain directions. Then, a x d = c and c x a = b, where a, b, and c are the principal material axes.

> FHWA-HRT-04-097

TFHRC Home | FHWA Home | FeedbackUnited States Department of Transportation - Federal Highway Administration

5 of 5

16.12.2009 15:06

Section 1.3. Elastic Constitutive Equations - Manual for LS-DYNA Wo...

http://www.tfhrc.gov/safety/pubs/04097/sec130.htm

TFHRC Home > Safety > FHWA-HRT-04-097 > Elastic Constitutive Equations

>

Manual for LS-DYNA Wood Material Model 1431.3 ELASTIC CONSTITUTIVE EQUATIONS1.3.1 Measured Clear Wood Moduli Wood guardrail posts are commonly made of southern yellow pine or Douglas fir. The clear wood moduli of southern yellow pine are given in table 1 in terms of the parallel and perpendicular directions. The parallel direction refers to the longitudinal direction. The perpendicular direction refers to the radial or tangential direction, or any normal stress measurement in the R-T plane. These properties were measured as a function of moisture content.(13) Moisture content is more thoroughly discussed in section 1.9. Table 1. Average elastic moduli of southern yellow pine. Moisture Content (%) 4 7 12 18 Saturated Modulus of Elasticity (MPa) Tension Parallel 16,469 15,559 15,503 12,283 11,283 Tension Perpendicular 959 1,000 552 297 Compression Parallel 18,345 17,469 16,572 11,690 7,959 Compression Perpendicular 848 766 593 414 221 Poissons Ratio LT LR

0.291 0.158 0.270 0.133 0.260 0.126 0.183 0.078 0.162 0.138

The clear wood moduli of Douglas fir are given in table 2 as a function of the longitudinal (parallel), tangential, and (15) radial directions. These properties were measured as a function of moisture content. Only compressive moduli were measured. Table 2. Average elastic moduli of Douglas fir. Moisture Content (%) 7 13 20 1.3.2 Review of Equations Wood materials are commonly assumed to be orthotropic because they possess different properties in three directionslongitudinal, tangential, and radial. The elastic stiffness of an orthotropic material is characterized by nine independent constants. The nine elastic constants are E11, E22, E33, G12, G13, G23, v12, v13, and v23, where E = Youngs modulus, G = shear modulus, and v = Poissons ratio. The general constitutive relationship for an orthotropic material, written in terms of the principal material directions(16) is: Modulus of Elasticity (MPa) Compression Longitudinal 16,345 16,414 15,193 Compression Tangential 993 779 483 Compression Radial 959 1,062 166 Poissons Ratio LT LR TR

0.441 0.295 0.368 0.449 0.292 0.374 0.496 0.274 0.396

1 of 3

16.12.2009 15:01

Section 1.3. Elastic Constitutive Equations - Manual for LS-DYNA Wo...

http://www.tfhrc.gov/safety/pubs/04097/sec130.htm

Subscripts 1, 2, and 3 refer to the longitudinal, tangential, and radial stresses and strains (s1 = s11, s2 = s22, s3 = s33, e1 = e11, e2 = e22, and e3 = e33, respectively). Subscripts 4, 5, and 6 are a shorthand notation that refers to the shearing stresses and strains (s4 = s12, s5 = s23, s6 = s13, e4 = e12, e5 = e23, and e6 = e13). As an alternative notation for wood, it is common to substitute L (longitudinal) for 1, R (radial) for 2, and T (tangential) for 3. The components of the constitutive matrix, Cij, are listed here in terms of the nine independent elastic constants of an orthotropic material:

The following identity, relating the dependent (minor Poissons ratios v21, v31, and v32) and independent elastic constants, is obtained from symmetry considerations of the constitutive matrix:

Another common assumption is that wood materials are transversely isotropic. This means that the properties in the tangential and radial directions are modeled the same (i.e., E22 = E33, G12 = G13, and v12 = v13). This reduces the number of independent elastic constants to five: E11, E22, v12, G12, and G23. Furthermore, the Poissons ratio in the isotropic plane, v23, is not an independent quantity. It is calculated from the isotropic relationship v = (E 2G)/2G, where E = E22 = E33 and G = G23. Transverse isotropy is a reasonable assumption if the difference between the tangential and radial properties is small in comparison with the difference between the tangential and longitudinal properties. The wood model formulation is transversely isotropic because the clear wood data in table 1 for southern yellow pine do not distinguish between the tangential and radial moduli. In addition, the clear wood data for Douglas fir in table 2 indicate that the difference between the tangential and radial moduli is less than 2 percent of the longitudinal modulus.

2 of 3

16.12.2009 15:01

Section 1.3. Elastic Constitutive Equations - Manual for LS-DYNA Wo...

http://www.tfhrc.gov/safety/pubs/04097/sec130.htm

1.3.3 Default Elastic Stiffness Properties Room-temperature moduli at saturation (23-percent moisture content) are listed in table 3. The same stiffnesses are used for graded wood as for clear wood. For southern yellow pine, the default Youngs moduli are average tensile values obtained from empirical fits to the clear wood data given in table 1 and shown in appendix B. These fits were published by FPL.(13) For Douglas fir, the default Youngs moduli and Poissons ratios are also obtained from empirical fits, made by the contractor, to the clear wood data given in table 2. The shear moduli were not measured. For both wood species, the parallel shear modulus is estimated from predicted elastic parameter tables for softwoods found in Bodig and Jayne.(16) The perpendicular shear modulus, G23, is calculated from the isotopic relationship between G23, E22, and v23. For both wood species, the value of the perpendicular Poissons ratio used to estimate G23 is that measured for Douglas fir (because no values are listed in table 1 for pine). Table 3. LS-DYNA default values for the room-temperature moduli (graded or clear wood) of southern yellow pine and Douglas fir at saturation. Southern Yellow Pine E11 or EL E22 or ET G12 or GLT G23 or GTR v12 or vLT 1.3.4 Orientation Vectors Because the wood model is transversely isotropic, the orientation of the wood specimen must be set relative to the global coordinate system of LS-DYNA. The transversely isotropic constitutive relationships of the wood material are developed in the material coordinate system (i.e., the parallel and perpendicular directions). The user must define the orientation of the material coordinate system with respect to the global coordinate system. Appropriate coordinate transformations are formulated in LS-DYNA between the material and global coordinate systems. Such coordinate transformations are necessary because any differences between the grain axis and the structure axis can have a great effect on the structural response. Keep in mind that the wood grain axis may not always be perfectly aligned with the wood post axis because trees do not always grow straight. It is up to the analyst to set the alignment of the grain relative to the wood post in LS-DYNA simulations. > FHWA-HRT-04-097 TFHRC Home | FHWA Home | FeedbackUnited States Department of Transportation - Federal Highway Administration

Douglas Fir 15,190 MPa 324 MPa 784 MPa 116 MPa 0.39

11,350 MPa 247 MPa 715 MPa 88 MPa 0.16

3 of 3

16.12.2009 15:01

Section 1.4. Failure Criteria - Manual for LS-DYNA Wood Material M...

http://www.tfhrc.gov/safety/pubs/04097/sec140.htm

TFHRC Home > Safety > FHWA-HRT-04-097 > Failure Criteria

>

Manual for LS-DYNA Wood Material Model 1431.4 FAILURE CRITERIAStrength variations are readily modeled with failure criteria, which are also called yield criteria. Failure criteria relate critical combinations of stresses or strains to failure in a material. Two types of failure criteria are limit and interactive criteria. With limit criteria, like the Maximum Stress criterion, there is no interaction between the stresses, so failure depends on one component of stress or strain. With interactive criteria, like the Hashin criterion, the stresses interact, so failure depends on more than one component of stress or strain. The failure stresses/strains for the interactive and maximum stress/strain criteria typically agree in the material principal directions (uniaxial stress states). The criteria disagree on what constitutes failure in off-axis directions (biaxial and triaxial stress states). 1.4.1 Measured Clear Wood Strengths Failure criteria are formulated with coefficients that are obtained from fits to measured strengths (peak strength in tension and shear, yield strength in compression). The clear wood strengths of southern yellow pine are given in table 4 in terms of the parallel, perpendicular, and shear directions. The shear strength refers to the parallelto-the-grain direction. No shear strength was reported for the perpendicular-to-the-grain direction because it is difficult to measure and interpret. The modulus of rupture is calculated from the beam-bending test results, in which the grain runs parallel to the length of the beam. It is not an input parameter of the wood material model. These strengths were measured as a function of moisture content.(13) The saturated data are measured at the fiber saturation point of approximately 23-percent moisture content. Table 4. Average strength data for southern yellow pine. Modulus Moisture Tension Tension Compression Compression Shear of Content Parallel Perpendicular Parallel Perpendicular Parallel Rupture (%) MPa) (MPa) (MPa) (MPa) (MPa) (MPa) 4 7 12 18 Saturated 119 136 146 134 101 3.96 4.26 4.50 3.38 1.86 76.7 66.8 52.0 33.1 21.5 14.8 13.0 10.0 7.3 4.0 19.9 19.2 16.8 13.5 8.9 129 121 107 76 49

The clear wood strengths of Douglas fir are given in table 5. These strengths were obtained from a variety of sources. No single source provides a complete set of strengths. Some sources distinguish between the radial and tangential directions, while others report strengths in the perpendicular direction. Whenever perpendicular strengths were reported, they were listed under the subheading Tangential for the normal strengths and LT for the shear strengths.

1 of 3

16.12.2009 15:02

Section 1.4. Failure Criteria - Manual for LS-DYNA Wood Material M...

http://www.tfhrc.gov/safety/pubs/04097/sec140.htm

Table 5. Average strength data for Douglas fir. Source Strength (MPa) Goodman and (7) Bodig (12%) Woodward and (17) Minor (12%) USDA Handbook(18) (Green) USDA Handbook(18) (12-13%) PattonMallory, (19) et al.

Tension Longitudinal Tangential Radial Compression Longitudinal Tangential Radial Shear LT LR RT 5.4 7.5 9.0 7.7 6.6 9.7 8.1 51.9 5.1 4.3 23.9 2.5 47.6 5.3 45.2 123.1 3.8 107.6 2.3 2.7 156.6 3.2 -

2 of 3

16.12.2009 15:02

Section 1.5. Plastic Flow - Manual for LS-DYNA Wood Material Mode...

http://www.tfhrc.gov/safety/pubs/04097/sec150.htm

TFHRC Home > Safety > FHWA-HRT-04-097 > Plastic Flow

>

Manual for LS-DYNA Wood Material Model 1431.5 PLASTIC FLOWThe plasticity algorithms limit the stress components once the failure criterion in equations 13 or 14 is satisfied. 1 This is done by returning the stress state back to the yield surface. Our traditional approach for modeling plasticity is to partition the stress and strain tensors into elastic and plastic parts. Partitioning is done with return mapping algorithms that enforce the plastic consistency conditions. Such algorithms allow one to control plastic strain generation. In addition, return mapping algorithms with associated flow satisfy the second law of thermodynamics. Associated flow is discussed in appendix D. Two simple types of plasticity algorithms are those that reduce the moduli directly and those that scale back the stresses directly. Although simple to implement, such methods do not allow one to control plastic strain generation and do not necessarily satisfy the second law of thermodynamics. 1.5.1 Consistency Parameter Updates Separate plasticity algorithms are modeled for the parallel and perpendicular modes by enforcing separate consistency conditions. Each consistency condition is derived in appendix D. The solution of each consistency condition determines the consistency parameters Dl and Dl^. The Dl solutions, in turn, determine the stress updates. Parallel Modes The parallel failure criterion from equation 13 is redefined as f|| (I1, I4) 0, with:1

where I1 and I4 are two of the five invariants of a transversely isotropic material. In this case, the expression Dl|| is:

Dl|| is calculated from specification of the total strain increments and the yield function

. The

trial elastic stress invariants, and , are calculated from the trial elastic stresses (see section 1.5.2). For the failure surface function in equation 15, the partial derivatives in equation 16 are:

1 of 3

16.12.2009 15:03

Section 1.5. Plastic Flow - Manual for LS-DYNA Wood Material Mode...

http://www.tfhrc.gov/safety/pubs/04097/sec150.htm

Perpendicular Modes The perpendicular failure criterion from equation 14 is redefined as f^ (I3, I4) 0, with:

where I2 and I3 are two of the five invariants of a transversely isotropic material. In this case, the expression for Dl^ is:

Dl^is calculated from specification of the total strain increments and the yield function

, where

and are the trial elastic stress invariants. For the failure surface function in equation 21, the partial derivatives in equation 22 are:

1.5.2 Elastoplastic Stress Updates The stresses are readily updated from the total strain increments and the consistency parameters:

where: n = nth time step in the finite element analysis s*ij = trial elastic stress updates calculated from the total strain increments, Deij, prior to application of plasticity

2 of 3

16.12.2009 15:03

Section 1.5. Plastic Flow - Manual for LS-DYNA Wood Material Mode...

http://www.tfhrc.gov/safety/pubs/04097/sec150.htm

Total strain increments are calculated by the finite element code from the dynamic equations of motion and the time step. Each normal stress update depends on the consistency parameters and failure surface functions for both the parallel (Dl = Dl|| and f = f||) and perpendicular (Dl = Dl^ and f = f^) modes. Each shear stress update depends on just one consistency parameter and failure surface function. If neither parallel nor perpendicular yielding occurs and , then Dl = 0 and the stress update is trivial: .

For the stress updates in equation 27, the partial derivatives are:

> FHWA-HRT-04-097

TFHRC Home | FHWA Home | FeedbackUnited States Department of Transportation - Federal Highway Administration

3 of 3

16.12.2009 15:03

Section 1.6. Hardening - Manual for LS-DYNA Wood Material Model ...

http://www.tfhrc.gov/safety/pubs/04097/sec160.htm

TFHRC Home > Safety > FHWA-HRT-04-097 > Hardening

>

Manual for LS-DYNA Wood Material Model 1431.6 HARDENINGWood exhibits prepeak nonlinearity in compression parallel and perpendicular to the grain. Perpendicular hardening was previously demonstrated in figure 3(b) for clear pine. A choice was made between two possible approaches for modeling prepeak nonlinearity. The first approach was to model bilinear hardening behavior by specifying initial and hardening moduli. This approach simulates a sudden change in modulus. However, real data, such as that previously shown in figure 3(b), exhibits a gradual change in modulus. The second approach was to model a translating yield surface that simulates a gradual change in modulus. This is the chosen approach. 1.6.1 Model Overview Our approach is to define initial yield surfaces that harden (translate) until they coincide with the ultimate yield surfaces, as demonstrated in figure 13 for the parallel modes. Separate formulations are modeled for the parallel and perpendicular modes. The initial location of the yield surface determines the onset of plasticity. The rate of translation determines the extent of nonlinearity.

1 of 5

16.12.2009 15:03

Section 1.6. Hardening - Manual for LS-DYNA Wood Material Model ...

http://www.tfhrc.gov/safety/pubs/04097/sec160.htm

Figure 13. Prepeak nonlinearity is modeled in compression with translating yield surfaces that allow user to specify the hardening response. For each mode (parallel and perpendicular), two hardening parameters must be defined. The first parameter, N, determines the onset of nonlinearity of the load-deflection or stress-strain curves. For example, consider the case where the user wants prepeak nonlinearity to initiate at 60 percent of the peak strength. The user inputs N = 0.4 so that 1 N = 0.6. The second parameter, c, determines the rate of hardening(i.e.,how rapidly or gradually the load-deflection or stress-strain curves harden). If the user wants rapid hardening, then a large value of c is input (e.g., c = 1000). If the user wants gradual hardening, then a small value of c is input (e.g., c = 10). The value of c needed for any particular fit depends on the properties of the material being modeled. It is selected by running

2 of 5

16.12.2009 15:03

Section 1.6. Hardening - Manual for LS-DYNA Wood Material Model ...

http://www.tfhrc.gov/safety/pubs/04097/sec160.htm

simulations (single-element simulations are fastest) with various values of c and comparing those simulations with data. Hardening model equations are given in section 1.6.3. In addition to modeling prepeak nonlinearity as shown in figure 13, a separate formulation models postpeak hardening, as shown in figure 14. Instead of coinciding with the ultimate yield surface, the initial yield surface passes through the ultimate yield surface. The larger the value of the input parameter Ghard,the more pronounced the postpeak hardening. A zero value for Ghard will produce perfectly plastic behavior. The default value is zero. Currently, Ghard controls both the parallel and perpendicular behaviors simultaneously.

Figure 14. Postpeak hardening is modeled in compression with positive values of the parameter Ghard. 1.6.2 Default Hardening Parameters Default hardening parameters for clear wood pine and fir are given in table 7. These hardening parameters were set by the contractor by correlating LS-DYNA simulations with compression tests conducted on 15- by 15- by 305-centimeter (cm) timbers.(2) Values of N|| = 0.5 and N^ = 0.4 were fit to the timber compression data for parallel and perpendicular behavior, respectively. These values for N|| and N^ are independent of grade, temperature, and moisture content. Values for c|| and c^ depend on the wood grade, but are independent of temperature and moisture content. Good fits to the data were obtained with the following formulas:

Qc = compression strength-reduction factor for graded wood discussed in section 1.12. Table 7. Default hardening parameters for clear wood southern yellow pine and Douglas fir. Parallel Wood N|| Southern Yellow Pine Douglas Fir 1.6.3 Hardening Model Theory Parallel Modes 0.5 0.5 c|| 400 400 N^ 0.4 0.4 c^ 100 100 Perpendicular

3 of 5

16.12.2009 15:03

Section 1.6. Hardening - Manual for LS-DYNA Wood Material Model ...

http://www.tfhrc.gov/safety/pubs/04097/sec160.htm

The state variable that defines the translation of the yield surface is known as the backstress and is denoted by aij. Prepeak nonlinearity is modeled in compression, but not shear, so the only backstress required for the parallel modes is a11. The value of the backstress is a11 = 0 upon initial yield and a11 = N||Xc at ultimate yield (in uniaxial compression). The maximum backstress occurs at ultimate yield and is equal to the total translation of the yield surface in stress space. The hardening rule defines the growth of the backstress. Hardening rules are typically based on stress or plastic strain. Hardening is based on stress. This is accomplished by defining the incremental backstress:

where: c|| = user input parameter that determines rate of translation G|| = function that properly limits the increments s11 a11 = reduced stress that determines direction of translation (longitudinal) = effective strain-rate increment parallel to the grain Dt = time step These terms are internally calculated by the material model and LS-DYNA, and are included to keep the hardening response independent of time step, time-step scale factor, and strain increment. The effective strain rate is a scalar value that is equal to:

The function G|| restricts the motion of the yield surface so that it cannot translate outside the ultimate surface.(20) The functional form of G|| is determined from the functional form of the yield surface and the longitudinal stress definition. A brief derivation is given in appendix E. Thus, it is defined as:

The value of the limiting function is G||= 1 at initial yield (because a11 = 0) and G||= 0 at ultimate yield (because ). Thus, G|| limits the growth of the backstress as the ultimate surface is approached. If postpeak a11 = N|| hardening is active, then the minimum value is maintained at G||= Ghard rather than G||= 0. The ultimate yield surface is defined from equation 13 as:

For the case of uniaxial compressive stress (no shear), the ultimate yield surface reduces to Perpendicular Modes

= Xc.

Prepeak nonlinearity is modeled in compression, but not shear, so the backstress components required are a22 and a33. The value of the backstress sum is a22 + a33 = 0 upon initial yield and a22 + a33 = N^Yc at ultimate yield (biaxial compression without shear). The backstress increments are defined as follows:

where: c^ = user input parameter that determines rate of translation

4 of 5

16.12.2009 15:03

Section 1.6. Hardening - Manual for LS-DYNA Wood Material Model ...

http://www.tfhrc.gov/safety/pubs/04097/sec160.htm

= effective strain-rate increment perpendicular to the grain:

The functional form of G^ is determined from the functional form of the yield surface in equation 14 as:

The value of G^ ranges from 1 at initial yield to 0 at ultimate yield. If postpeak hardening is active, then the minimum value is G^= Ghard rather than G^= 0. The ultimate yield surface is defined from equation 14 as:

Consider the case of biaxial compressive stress (I3 = 0). Initially, a22 + a33 = 0, so G^ = 1. Ultimately, a22 + a33 = N^Yc and = s22 + s33 = Yc, so G^ = 0.

1.6.4 Implementation Aspects The plasticity model discussed in the section 1.5 is modified to account for compressive hardening. Modifications are made to the failure surface definitions and the stress updates. Failure Surface Definitions With Hardening For the parallel modes, initial yielding occurs when f|| > 0, with:

For the perpendicular modes, initial yielding occurs when f^ > 0, with:

No modifications are necessary for the tensile modes. Stress and Backstress Updates Total stress is updated from the sum of the initial yield stress plus the backstress:

> FHWA-HRT-04-097

TFHRC Home | FHWA Home | FeedbackUnited States Department of Transportation - Federal Highway Administration

5 of 5

16.12.2009 15:03

Section 1.7. Postpeak Softening - Manual for LS-DYNA Wood Materia...

http://www.tfhrc.gov/safety/pubs/04097/sec170.htm

TFHRC Home > Safety > FHWA-HRT-04-097 > Postpeak Softening

>

Manual for LS-DYNA Wood Material Model 1431.7 POSTPEAK SOFTENINGIn addition to predicting the critical combination of stresses at failure, modeling post-failure degradation of these stresses (softening) is particularly important. Postpeak degradation occurs in the tensile and shear modes of wood. This was previously demonstrated in figure 3. 1.7.1 Degradation Model Degradation models are used to simulate postpeak softening. A choice was made between simple and sophisticated approaches for modeling degradation. Simple degradation models fit into one of three categories: instantaneous unloading, gradual unloading, and no unloading (constant stress after yielding, as modeled with plasticity). Although tensile and parallel shear failures are brittle, instantaneous unloading over one time step would cause dynamic instabilities. An alternative is to gradually unload over a number of time steps. Although simple to implement, such an ad hoc treatment will produce mesh-size dependency. This means that the same physical problem will produce different results for different mesh configurations. Two other disadvantages of these formulations are: (1) stiffness is not degraded in conjunction with strength and (2) progressive softening is independent of subsequent loading. Both of these behaviors are unrealistic. A more sophisticated approach is to model degradation with a damage formulation. A scalar damage parameter, d, transforms the stress tensor associated with the undamaged state, the damaged state, sij: , into the stress tensor associated with

The stress tensor is calculated by the plasticity and viscoplasticity algorithms prior to application of the damage model. The damage parameter ranges from zero for no damage to approaching unity for maximum damage. Thus, 1 d is a reduction factor associated with the amount of damage. A distinct advantage of damage formulations over ad hoc formulations is that they degrade stiffness in conjunction with strength. Experimental evidence for stiffness degradation was previously shown in equation 16. In addition, progressive degradation does not occur over one time step; it depends on subsequent loading (stress spikes and transient waves will not cause spurious early failures because the load is not sustained). However, mesh-size dependency is still an issue and is discussed in section 1.7.2. This is the chosen approach. Damage Parameter Functional Form Two damage formulations are implemented for modeling degradation of wood: one formulation for the parallel modes and a separate model for the perpendicular modes: Parallel Modes

Perpendicular Modes

For each formulation, damage is specified by three user-supplied parameters. For the parallel modes, these

1 of 11

16.12.2009 15:04

Section 1.7. Postpeak Softening - Manual for LS-DYNA Wood Materia...

http://www.tfhrc.gov/safety/pubs/04097/sec170.htm

parameters are A,B, and parameter

. For the perpendicular modes, these parameters are C,D, and

. The

limits the maximum level of damage. It ranges between 0 and 1. No damage accumulates if

=0. Typically, 1, which means that the maximum damage level attained is d1. This, in turn, means that the stiffness and strength are ultimately degraded to zero. The evolution of the damage parameter d is shown in figure 15 as a function of t. The strain-based energy term t is calculated by the model. Its analytical form for both the parallel and perpendicular modes is discussed in subsequent paragraphs. Damage accumulates when t exceeds an initial damage threshold t0. Four curves are shown in figure 15 that correspond to four sets of softening parameters, C and D. The parameter C sets the midslope of the curve near d = 0.5 (larger values of C produce larger midslopes). The parameter D sets the initial slope near the threshold (smaller values of D produce larger initial slopes). Here, t0 0.055.

Figure 15. Damage d accumulates with energy t once an initial threshold t0 is exceeded. Softening is demonstrated in figure 16 for tensile failure perpendicular to the grain. Four softening curves are shown, which correspond to the four sets of softening parameters previously used in figure 15. The parameters C and D shape the softening curve. Larger values of D produce a flatter peak. Larger values of C produce more severe softening.

2 of 11

16.12.2009 15:04

Section 1.7. Postpeak Softening - Manual for LS-DYNA Wood Materia...

http://www.tfhrc.gov/safety/pubs/04097/sec170.htm

Figure 16. Softening depends on the values of the damage parameters C and D(calculated with dmax = 1). Damage Parameter Strain Basis Damage formulations are typically based on strain, stress, or energy. The wood model bases damage accumulation on the history of strains. One of the more famous strain-based theories is that proposed by Simo and Ju for modeling damage in isotropic materials such as concrete.(21) They base damage on the total strains and the undamaged elastic moduli. They do this by forming the undamaged elastic strain energy norm, . For simplicity, 2 we have defined elasticity tensor previously given in equation 1. One way of expanding t is: where Cijkl is the linear

2

The stress tensor

is not equal to the elasto-viscoplastic stress tensor

nor to the damaged

elastoplastic stress tensor convenience.

. It is a fictitious stress that is based on the total strain and is defined for

Separate strain energy norms are implemented for modeling damage accumulation in the parallel and perpendicular modes. Parallel Modes Damage in the parallel modes is based on the following strain energy norm:

Wood is being treated as transversely isotropic; therefore, t|| was chosen to be the portion of the undamaged elastic strain energy that is associated with the parallel modes (specific terms from equation 51 were retained that contain the parallel normal and shear strains). Damage accumulates when t|| exceeds . The initial

3 of 11

16.12.2009 15:04

Section 1.7. Postpeak Softening - Manual for LS-DYNA Wood Materia...

http://www.tfhrc.gov/safety/pubs/04097/sec170.htm

threshold is not a user-supplied parameter. It is calculated and permanently stored by the wood material model at the time that the parallel failure criterion is first satisfied in tension. Damage accumulates in both the tensile and parallel shear modes, but not the compressive mode. Perpendicular Modes Damage in the perpendicular modes is based on the following strain energy norm:

The term t^ was chosen to be the portion of the undamaged elastic strain energy that is associated with the perpendicular modes (specific terms from equation 51 are retained that contain the perpendicular normal and . The initial threshold is not a user-supplied shear strains). Damage accumulates when t^ exceeds parameter; it is calculated and permanently stored by the wood material model once the perpendicular failure criterion is satisfied in tension. Damage accumulates in both the tensile and perpendicular shear modes, but not in the compressive mode. Strength Coupling Another issue is strength coupling, in which degradation in one direction affects degradation in another direction. If failure occurs in the parallel modes, then all six stress components are degraded uniformly. This is because parallel failure is catastrophic and will render the wood useless. The wood is not expected to carry load in either the parallel or perpendicular directions once the wood fibers are broken. If failure occurs in the perpendicular modes, then only the perpendicular stress components are degraded. This is because perpendicular failure is not catastrophic (the wood is expected to continue to carry the load in the parallel direction). Based on these assumptions, the following degradation model is implemented:

1.7.2 Regulating Mesh-Size Dependency If a model is mesh-size dependent, then different mesh refinements produce different computational results. This is undesirable and is the result of modeling element-to-element variation in the fracture energy instead of modeling uniform fracture energy. Fracture energy is the area under the stress-displacement curve in the softening regime. If the fracture energy is not constant from element to element, then excess damage will accumulate in the smallest elements because the fracture energy is less in the smaller elements. Regulatory methods eliminate this variation and the excess damage accumulation. Fracture energy is a property of a material and special care must be taken to treat it as such. There are a number of approaches for regulating mesh-size dependency. One approach is to manually adjust the damage parameters as a function of element size to keep the fracture energy constant. However, this approach is not practical because the user would have to input different sets of damage parameters for each size element. A more automated approach is to include an element-length scale in the model. This is done by passing the element

4 of 11

16.12.2009 15:04

Section 1.7. Postpeak Softening - Manual for LS-DYNA Wood Materia...

http://www.tfhrc.gov/safety/pubs/04097/sec170.htm

size through to the wood material model and internally calculating the damage parameters as a function of element size. Finally, viscous methods for modeling rate effects also regulate mesh-size dependency. However, if rate-independent calculations are performed, then viscous methods will be ineffective. The wood model regulates mesh-size dependency by explicitly including the element size in the model. The element size is calculated as the cube root of the element volume. Softening in the parallel and perpendicular modes is regulated separately because different fracture energies are measured in the parallel and perpendicular modes. Parallel Mode Regularization The relationship between the parallel fracture energy, Gf||; the softening parameters, A and B; and the element size, L, is:

This expression for the fracture energy was derived by integrating the analytical stress-displacement curve:

where: x = displacement x0 = displacement at peak strength, XT To accomplish the integration, the damage threshold difference is related to the stiffness and displacement as

follows:

. In addition, the functional form of d is given by equation 49 with dmax = 1.

To regulate mesh-size dependency, the wood model requires values for B, , and , rather than A and B. When the parallel failure criterion is satisfied, the wood material model internally solves equation 62 for the value of A based on the initial element size, initial damage threshold, and fracture energy for the particular mode of parallel failure that is initiated (tensile, shear, or compressive):

The fracture energy varies with failure mode in the following manner:

When failure is entirely tensile (s11 = XT, s12 = s13 = 0), then piecewise function of tension fracture energy and softening is brittle. When failure is entirely shear , then and softening is more gradual. When failure is compressive (s11 = XC,s12 = s13 = 0),thenGf = and no softening occurs. Example stress-strain curves for these failure modes are given in figure 17. They were calculated for the default clear wood moduli and strengths at 12-percent moisture content. Default hardening and fracture energies, however, were not set at the time these figures were created. The parallel fracture energies simulated are seven times the perpendicular fracture energies. Perpendicular Mode Regularization

5 of 11

16.12.2009 15:04

Section 1.7. Postpeak Softening - Manual for LS-DYNA Wood Materia...

http://www.tfhrc.gov/safety/pubs/04097/sec170.htm

An expression similar to equation 62 is readily obtained for the fracture energy perpendicular to the grain:

To regulate mesh-size dependency, the wood model requires input values for D, C and D.

, and

, rather than

When the perpendicular failure criterion is satisfied, the wood material model internally solves equation 66 for the value of C based on the initial element size, initial damage threshold, and fracture energy for the particular mode of perpendicular failure that is initiated (tensile, shear, or compressive):

Fracture energy varies with failure mode in the following manner:

When failure is entirely tensile (s22 + s33 = YT, s23 = 0), then is entirely shear When failure is compressive , then

and softening is brittle. When failure and softening is more gradual. , then Gf = and no softening occurs.

Stress-strain curves for these failure modes are given in figure 18. They were calculated for the default moduli, strengths, and fracture energies at 12-percent moisture content.

6 of 11

16.12.2009 15:04

Section 1.7. Postpeak Softening - Manual for LS-DYNA Wood Materia...

http://www.tfhrc.gov/safety/pubs/04097/sec170.htm

Figure 17. Softening response modeled for parallel modes of southern yellow pine.

7 of 11

16.12.2009 15:04

Section 1.7. Postpeak Softening - Manual for LS-DYNA Wood Materia...

http://www.tfhrc.gov/safety/pubs/04097/sec170.htm

Figure 18. Softening response modeled for perpendicular modes of southern yellow pine. 1.7.3 Default Damage Parameters

The damage model requires input of eight damage parametersfour for the parallel modes (B,

,

,

and dmax||) and four for the perpendicular modes (D, , , and dmax^). Default values for the maximum damage parameters are dmax|| = 0.9999 and dmax^ = 0.99. These values are slightly less than 1. This is to avoid potential computational difficulties associated with zero stiffness for dmax = 1. In addition, the parallel

8 of 11

16.12.2009 15:04

Section 1.7. Postpeak Softening - Manual for LS-DYNA Wood Materia...

http://www.tfhrc.gov/safety/pubs/04097/sec170.htm

damage parameter is closer to 1 than the perpendicular parameter. This is because elements erode with maximum parallel damage, but not with maximum perpendicular damage (see section 1.7.4). One percent of the original perpendicular stiffness and strength is retained to avoid computational difficulties. Default shape parameters are B = D = 30. Data are not available to set the shape of the softening curves, so they have been arbitrarily chosen. Default fracture energies are based on the FPL data reported in appendix A for fracture intensities. Fracture energies are derived from the fracture intensities, as discussed in subsequent paragraphs. Default values for all eight input parameters are given in table 8 for room-temperature clear wood pine and fir at saturation. Table 8. LS-DYNA default values for room-temperature clear wood softening parameters for southern yellow pine and Douglas fir at saturation. Perpendicular D (MPa.cm) Pine Fir 30 30 0.0210 0.0210 (MPa.cm) 0.0788 0.0788 0.99 0.99 30 30 dmax^ B (MPa.cm) 2.2344 2.2344 (MPa.cm) 8.3843 8.3843 0.9999 0.9999 Parallel dmax||

Fracture energies for Douglas fir are set equal to those for southern yellow pine. This is because fracture intensity data are not available for Douglas fir, and grade 1 bogie-post impact simulations correlated with test data suggest that this assumption is reasonable.(2) Measured Fracture Intensities The effect of moisture content on the mode I and mode II fracture intensities of southern yellow pine is given in table 9 for the perpendicular modes. These data were measured with the load applied in the tangential direction and the crack propagation in the longitudinal direction.(13) Fracture intensities were measured from compacttension specimens (7.62 by 8.26 by 2.0 cm) and center-split beams (65 by 6 by 2 cm). No data are reported for the parallel modes. Published data indicate that the mode I fracture intensities measured parallel to the grain are 3(16) about seven times those measured perpendicular to the grain.3

Personal communication with Dr. David Kretschmann of FPL. Table 9. Average fracture intensity data for southern yellow pine measured perpendicular to the grain. Moisture Content (%) 4 7 12 18 Saturated KI (MPa-cm1/2) 4.69 5.03 4.66 3.85 2.85 KII (MPa-cm1/2) 18.54 20.41 20.65 18.39 13.71

Derived Fracture Energies The mode I and mode II fracture energies are related to the fracture intensities through the following analytical expressions:

where: (22) C| and C|| = constants related to the moduli of an orthotropic material:

9 of 11

16.12.2009 15:04

Section 1.7. Postpeak Softening - Manual for LS-DYNA Wood Materia...

http://www.tfhrc.gov/safety/pubs/04097/sec170.htm

Here, the compliance coefficients, Sij, are the reciprocals of the elastic moduli:

The values of C| and C|| vary with moisture content because moduli vary with moisture content (see appendix B). Tensile and shear perpendicular fracture energies as a function of moisture content are derived from equation 69 and FPLs quadratic equations for fracture intensity as a function of moisture content. Default fracture energies at saturation are given in table 10 for the perpendicular modes of pine and fir. These values are default values regardless of the grade or temperature of the wood. No fracture intensity or energy data are available for the parallel modes, so default values are based on LS-DYNA bogie-post impact simulations correlated with test data.(2) Correlations were made for grade 1 pine and fir posts, DS-65 pine posts, and frozen grade 1 pine posts. Good room-temperature grade 1 correlations (pine and fir) are obtained when the fracture energy parallel to the grain is 50 times greater than the fracture energy perpendicular to the grain. This parallel-to-perpendicular factor of 50 for energy is consistent with a parallel-to-perpendicular factor of 7 for intensity once equation 69 is applied (72 50).(16) In addition, good DS-65 correlations are obtained with a factor of 85, which indicates that the parallel fracture energy depends on the grade. To accommodate variation with grade, the default parallelto-the-grain fracture energies are modeled as:

Table 10. Room-temperature clear wood fracture energies for southern yellow pine and Douglas fir as a function of moisture content (derived from measured fracture intensities). Perpendicular Moisture Content (%) (MPa.cm) 4 7 12 18 Saturated 0.0204 0.0227 0.0225 0.0219 0.0210 (MPa.cm) 0.0768 0.0945 0.1028 0.1035 0.0788 (MPa.cm) 2.171 2.415 2.394 2.330 2.2344 (MPa.cm) 8.172 10.055 10.938 11.012 8.384 Parallel

These equations indicate that the default fracture energy of clear wood, parallel to the grain, is 106 times greater than the default fracture energy perpendicular to the grain. Default fracture energies derived from the above equations are given in table 10 for the parallel modes of pine and fir. 1.7.4 Modeling Breakaway Complete failure and breakup of a wood post is simulated with element erosion. 4 The erosion location is determined by the wood model from the physics of the problem. Dynamic instability is not an issue because the element erodes after it loses all strength and stiffness. In addition, mesh-size sensitivity is regulated through the

10 of 11

16.12.2009 15:04

Section 1.7. Postpeak Softening - Manual for LS-DYNA Wood Materia...

http://www.tfhrc.gov/safety/pubs/04097/sec170.htm

damage formulation. Parallel damage is catastrophic because cracking occurs across the grain, which breaks the fibers or tubular cells of the wood. An element will automatically erode if it fails in the parallel mode and the parallel damage parameter exceeds d|| = 0.99. Recall that default dmax|| = 0.9999, so the element erodes just prior to accumulating maximum damage. All six stress components are degraded with parallel damage, so the element loses nearly all strength and stiffness before eroding. If the user sets dmax|| < 0.99, then erosion will not occur. Perpendicular damage is not catastrophic because cracking occurs between the fibers, causing the wood to split at relatively low strength and energy levels. The fibers are not broken. An element does not automatically erode if it fails in the perpendicular mode. This is because only three (sR, sT, and sRT) of the six stress components are degraded with perpendicular damage. Since erosion does not automatically occur, dmax^ is set to 0.99 instead of 0.9999 so that the element retains 1 percent of its elastic stiffness and strength. In this way, computational difficulties associated with extremely low stiffness and strength will hopefully be avoided. As an option, a flag is available, which, when set, allows elements to erode when the perpendicular damage parameter exceeds d^ = 0.989. Setting this flag is not recommended unless excessive perpendicular damage is causing computational difficulties. As an additional precaution, an element will erode if d^ > 0.98, and the perpendicular normal and shear strains exceed a predefined value of 90 percent. Typically, erosion is more computationally efficient than the alternative approach of modeling fracture surfaces using tied surfaces with failure. One drawback of the tied surface approach is that an interface model (criteria) must be developed and validated for the tied nodes because the wood model is for elements, not interfaces. Another drawback is that the user must mesh the entire model with tied interfaces or else guess the failure location prior to running the calculation in order to specify the tied surface location. This is not practical. Other drawbacks are dynamic instability caused by sudden tied-node failure and mesh-size sensitivity. > FHWA-HRT-04-097 TFHRC Home | FHWA Home | FeedbackUnited States Department of Transportation - Federal Highway Administration

11 of 11

16.12.2009 15:04

Section 1.8. Rate Effects - Manual for LS-DYNA Wood Material Mode...

http://www.tfhrc.gov/safety/pubs/04097/sec180.htm

TFHRC Home > Safety > FHWA-HRT-04-097 > Rate Effects

>

Manual for LS-DYNA Wood Material Model 1431.8 RATE EFFECTSA number of approaches are available to accommodate strain-rate sensitivity. Simple approaches scale the input strengths or moduli as a function of strain rate. More sophisticated approaches use viscoplastic mechanisms. Viscoplastic mechanisms retard the development of plasticity, which allows the stress state to exceed the static failure surface. Viscoplastic mechanisms also increase the stiffness in conjunction with strength if plastic hardening is modeled in the prepeak regime. Both types of formulations are easy to implement and are computationally efficient. Therefore, two methods are implemented. One method scales each strength as a function of strain rate, effectively expanding the failure surface. The second method is viscoplastic. Both methods are discussed here. However, the shifted surface method is the easiest to fit, and it is the only method that has been validated to date, so it is the only active option in the wood model at this time. 1.8.1 High Strain-Rate Data A common test for measuring strain-rate effects is the split Hopkinson pressure bar (SHPB). Hopkinson bar data for pine are shown in figure 19.(11) Here, the dynamic-to-static stress ratio is plotted as a function of impact velocity for both the parallel and perpendicular directions. Rate effects are more pronounced in the perpendicular direction than in the parallel direction. Also plotted in figure 19 are theoretical curves derived from shock theory (i.e., conservation of mass and momentum across a shock front). The theoretical stress enhancement factors are:

where: = ratio of dynamic-to-static stress r = average wood density rs = wood solid phase density a = empirical shape factor for the stress-strain curve Values of rs = 1500 kilograms per square meter (kg/m2) and a = 1.35 are reported by Reid and Peng(11) for 2 wood and pine. For southern yellow pine with a density of r = 530 kg/m at 12-percent moisture content, the stress enhancement curves reduce to:

where V is measured in m/s. These curves indicate that the stress enhancement in the perpendicular direction is much greater than that in the

1 of 7

16.12.2009 15:04

Section 1.8. Rate Effects - Manual for LS-DYNA Wood Material Mode...

http://www.tfhrc.gov/safety/pubs/04097/sec180.htm

parallel direction. However, the curves tend to underestimate the stress enhancement, particularly at low-impact velocities (see figure 19). To fit the rate-effect model parameters, the stress enhancement ratios need to be derived as a function of strain rate. To do this, impact velocity must be converted to strain rate. However, Reid and Peng(11) did not report this conversion.

Figure 19. Hopkinson bar tests indicate that the measured strength of pine increases with impact velocity. (11) Source: Pergamon, Elsevier Science Ltd. Bragov and Lomunov also measured the dynamic properties of pine using the SHPB technique.(23) Stress-strain diagrams are depicted in figure 20. Data are measured parallel and perpendicular to the grain. In addition, two curve sets are shown for each direction, which correspond to two strain rates (approximately 1000 per second(s-1) and 500 s-1). The data indicate that both strength and parallel stiffness increase with strain rate.

Figure 20. Hopkinson bar data indicate that strength and stiffness increase with strain rate.

2 of 7

16.12.2009 15:04

Section 1.8. Rate Effects - Manual for LS-DYNA Wood Material Mode...

http://www.tfhrc.gov/safety/pubs/04097/sec180.htm

Source: EDP Sciences.(23) Parallel and perpendicular strength ratios versus strain rate are needed to fit the rate-effect model. Here, those ratios are estimated. Bragov and Lomunov report a static parallel compressive strength of XC = 41.4 MPa for (23) pine. This strength is used to calculate the parallel strength ratios from figure 20. Calculated values are (0) = 2.3 at 1000 per second (s) and (0) = 1.7 at 500/s. Bragov and Lomunov did not report a static (23) perpendicular compressive strength for YC. Therefore, one cannot directly estimate the perpendicular strength ratio from figure 20. Instead, the Reid and Peng velocity-strength ratio relationships in equation 76 are used to (11) estimate the impact velocities and perpendicular strength ratios. Impact velocities of 262 m/s and 192 m/s are derived from the parallel relationship in equation 76 for (0) = 2.3 and (0) = 1.7, respectively. Using these velocities, perpendicular strength ratios of (0) = 9.0 and (0) = 5.3 are derived from the perpendicular relationship in equation 76. These ratios are reported in table 11. Table 11. Strength ratios versus strain rate derived from compressive rate-effect data. Rate (s ) 0 500 1000 1.8.2 Shifted Surface Model Theory Separate rate-effect formulations are modeled for the parallel and perpendicular modes because the Reid and Peng data indicate that dynamic strength enhancement is more pronounced in the perpendicular direction than in (11) the parallel direction. The rate-effect formulations increase strength with increasing strain rate by expanding each yield surface: Parallel-1

(0) 1.0 1.7 2.3

(90) 1.0 5.3 9.0

Perpendicular

where: X and Y DYNAMIC DYNAMIC and Y X C h

= static strengths = dynamic strengths = excess stress components

Excess stress components depend on the value of the fluidity parameter, h; the stiffness, C; and the effective strain rate, . When rate effects are requested via the flag IRATE = 1, dynamic strengths are used in place of the static strengths in the yield surface formulations (in equations 13 and 14, or in equations 44 and 45). Four effective fluidity parameters are used (h||, hc||, h^, and hc^). Two parameters are needed for the parallel modesone for the tensile and shear strengths, and a second for the compressive strength. Two parameters are

3 of 7

16.12.2009 15:04

Section 1.8. Rate Effects - Manual for LS-DYNA Wood Material Mode...

http://www.tfhrc.gov/safety/pubs/04097/sec180.htm

also needed for the perpendicular modes. Each effective fluidity parameter is formulated from two input parameters:

The two-parameter formulation allows the user to model a nonlinear variation in dynamic strength with strain rate.(24) Setting n|| = 0 or n^ = 0 allows the user to model a linear variation in dynamic strength with strain rate. The total number of input parameters is six. Three parameters are input for the parallel modes (h||, hc||, and n||) and three parameters are input for the perpendicular modes (h||, hc||, and n^). Single-element simulations performed with and without rate effects (500/s) are shown in figure 21 for room-temperature clear wood at 12-percent moisture content. The dynamic-to-static strength ratio (0) = 1.7, previously listed in table 11, was used to set the rate-effect parameters for the compressive simulation. These parameters are given in table 12. The plots in figure 21 indicate that different dynamic-to-static strength ratios naturally occur for the tension simulations than for the compressive simulations, even though h|| = hc||. This is because the tensile and compressive simulations have the same excess stress components, but different static strengths.

Figure 21. These single-element simulations demonstrate the rate-effect behavior of the shifted surface formulation at 500/s. Table 12. Default LS-DYNA rate-effect parameters that provide the dynamic-to-static compressive strength ratios listed in table 11 (based on units of milliseconds for time) for pine at 12-percent moisture content. Parallel Wood h|| Pine Fir 0.0045 0.0045 hc|| 0.0045 0.0045 n|| 0.107 0.107 h^ 0.0962 0.0962 hc^ 0.0962 0.0962 n^ 0.104 0.104 Perpendicular

4 of 7

16.12.2009 15:04

Section 1.8. Rate Effects - Manual for LS-DYNA Wood Material Mode...

http://www.tfhrc.gov/safety/pubs/04097/sec180.htm

1.8.3 Viscoplastic Model Theory Viscoplastic algorithms allow the stress state to exceed the yield surface. The excess stress depends on the value of the fluidity parameter, h; the stiffness; and the strain rate. The viscoplastic (dynamic) stresses attained in uniaxial simulations are approximately those given in equations 77 through 82. Single- and two-parameter viscoplastic formulations are available. The single-parameter formulation was developed by Duvaut and Lions and models a linear variation in strength ratio with strain rate.(25) This is accomplished by specifying a constant value for each fluidity parameter (independent of strain rate). However, a linear variation is not necessarily appropriate for wood, as demonstrated in figure 19. A two-parameter (24) formulation was recently suggested by Murray to model a nonlinear variation in strength ratio with strain rate. The two-parameter formulation was previously given in equations 83 through 86. The viscoplastic formulation uses the same input parameters as the shifted surface formulation. The behavior of the viscoplastic model is shown in figure 22 for h = 0.0000094 s and four values of n. Here, the strength enhancement ratio (dynamic-to-static) has been plotted as a function of the strain rate. The smaller the value of n, the greater the strength enhancement at a given strain rate. The behavior of the two-parameter formulation reduces to that of the single-parameter formulation for n = 0. Thus, the Duvaut-Lions single-parameter model is a subset of the two-parameter model.

Figure 22. Two-parameter viscoplastic model is flexible in fitting data. The two-parameter viscoplastic update scheme is implemented as follows:

5 of 7

16.12.2009 15:04

Section 1.8. Rate Effects - Manual for LS-DYNA Wood Material Mode...

http://www.tfhrc.gov/safety/pubs/04097/sec180.htm

where: Dt and

= time step = viscid (dynamic) and inviscid (static) stress tensors, respectively = trial elastic stress

At each time step, and are calculated and saved by the plasticity algorithm. Then, equations 87 through 91 are applied to update the viscous solution. The inviscid and instantaneous elastic solutions are obtained as limiting cases of the implementation. This algorithm is easy to implement because the plasticity algorithm is not modified. The viscoplastic formulation is separate from and follows the plasticity algorithm. Separate formulations are implemented for the parallel (s11, s12, and s13) and perpendicular modes (s22, s33, and (11) s23), because the Reid and Peng test data suggest that the rate effects depend on grain orientation. The parallel stress components are updated with the parallel fluidity parameters, while the perpendicular stress components are updated with the perpendicular fluidity parameters. At this time, viscoplastic implementation requires only four parameters as input. These are h|| = hc|| and n|| for the parallel modes, and h^ = hc^ and n^ for the perpendicular modes. Therefore, one cannot specify separate dynamic overstresses for the tensile and compressive modes. Enhancement from four to six parameters could be conducted at a later date. Single-element simulations performed with and without viscoplastic rate effects (500/s) are shown in figure 23 for room-temperature clear wood pine at 12-percent moisture content, using the input parameters specified in table 12.5 The primary difference between the viscoplastic simulations and the shifted surface simulations (figure 21) is that the viscoplastic tensile simulation is nonlinear to peak, whereas the shifted surface simulation is linear. This is because plastic strains are being calculated with the viscoplastic formulation, not the shifted surface formulation. The user has no control over the linearity or nonlinearity with either formulation. Also note that the compressive simulations calculated with viscoplasticity attain the same dynamic peaks as those calculated with the shifted surface formulation. Different hardening parameters were used in each simulation, so the hardening is not identical. On the other hand, the tensile simulations calculated with the viscoplastic formulation attain lower peak strengths than those calculated with the shifted surface formulation. This is because damage accumulates in tension (not compression) and is applied to the stresses at the same time as viscoplasticity. Damage does not accumulate in tension during application of the shifted surface formulation. Default hardening and softening parameters were not finalized at the time that these plots were made, so these figures cannot be reproduced using the current default material property values. 1.8.4 Default Rate-Effect Parameters Default rate-effect parameters for the shifted surface formulation were previously given in table 12. They provide the strength enhancement ratios listed in table 11. No rate-effect data are available for Douglas fir, so the model uses the same default parameters as southern yellow pine. The viscoplastic algorithm uses four of the six shifted surface parameters (the compressive fluidity parameters are ignored).5

6 of 7

16.12.2009 15:04

Section 1.8. Rate Effects - Manual for LS-DYNA Wood Material Mode...

http://www.tfhrc.gov/safety/pubs/04097/sec180.htm

Figure 23. These single-element simulations demonstrate the rate-effect behavior of the viscoplastic formulation at 500/s. > FHWA-HRT-04-097 TFHRC Home | FHWA Home | FeedbackUnited States Department of Transportation - Federal Highway Administration

7 of 7

16.12.2009 15:04

Section 1.9. Model Input - Manual for LS-DYNA Wood Material Mode...

http://www.tfhrc.gov/safety/pubs/04097/sec190.htm

TFHRC Home > Safety > FHWA-HRT-04-097 > Model Input

>

Manual for LS-DYNA Wood Material Model 1431.9 MODEL INPUTThe previous eight subsections reviewed the behavior and properties of wood and the theory of the model. Here, we examine the effects of moisture content, temperature, and grade on model input parameters. Two methods are available for wood model input. One method is to provide the following input parameters: Five moduli for transversely isotropic constitutive equations. Six strengths for the yield criteria. Four prepeak hardening parameters. Eight postpeak softening parameters. Six rate-effect parameters. These 29 parameters are listed in table 13 and were discussed in detail throughout this section (Theoretical Manual). Any consistent system of units may be used. A second method is to request default material properties. Default material property requests are listed in table 14. This method is convenient because it allows the user to bypass the manual input of the material parameters. Default material properties are provided for southern yellow pine and Douglas fir as a function of moisture content, temperature, grade, and units. A discussion of the effects of moisture, temperature, and grade is given in the following three subsections. Four consistent sets of units are available. Most of the default material (14) properties are obtained from clear wood samples tested by FPL. In addition to the choice between user-supplied and default input parameters, the user may also specify control parameters. Control parameters include material identification, density, options to plot damage, increasing the maximum number of iterations performed by the plasticity algorithm, turning on/off the rate effects, overriding perfect plasticity, and controlling perpendicular erosion. Table 13. User-supplied parameters for wood material model. Parallel Normal Modulus Perpendicular Normal Modulus Moduli Parallel Shear Modulus Perpendicular Shear Modulus Parallel Major Poissons Ratio Parallel Tensile Strength Parallel Compressive Strength Parallel Shear Strength Strengths Perpendicular Compressive Strength Perpendicular Tensile Strength Perpendicular Shear Stren